# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_11
_database_code_depnum_ccdc_archive 'CCDC 2348857'
loop_
_audit_author_name
_audit_author_address
'Miriding Mutailipu'
;Chinese academic of science
China
;
_audit_update_record             
;
2024-04-17 deposited with the CCDC.	2024-05-02 downloaded from the CCDC.
;
_audit_creation_date             2021-10-10
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6408)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'B6 Cd4 O15 Sr2'
_chemical_formula_sum            'B6 Cd4 O15 Sr2'
_chemical_formula_weight         929.70
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   10.6878(11)
_cell_length_b                   5.2551(4)
_cell_length_c                   11.5527(12)
_cell_angle_alpha                90
_cell_angle_beta                 92.154(4)
_cell_angle_gamma                90
_cell_volume                     648.40(11)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    927
_cell_measurement_temperature    299.0
_cell_measurement_theta_max      27.44
_cell_measurement_theta_min      3.53
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    14.697
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5233
_exptl_absorpt_correction_type   none
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1042 before and 0.0645 after correction.
The Ratio of minimum to maximum transmission is 0.7019.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            COLORLESS
_exptl_crystal_density_diffrn    4.762
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       PLATE
_exptl_crystal_F_000             836
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0690
_diffrn_reflns_av_unetI/netI     0.0648
_diffrn_reflns_Laue_measured_fraction_full 0.974
_diffrn_reflns_Laue_measured_fraction_max 0.973
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            4541
_diffrn_reflns_point_group_measured_fraction_full 0.974
_diffrn_reflns_point_group_measured_fraction_max 0.973
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.511
_diffrn_reflns_theta_min         1.907
_diffrn_ambient_temperature      299.0
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.974
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_source_current           1.4
_diffrn_source_power             0.07
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                1229
_reflns_number_total             1455
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL  (Sheldrick, 2008)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_refine_diff_density_max         1.279
_refine_diff_density_min         -1.557
_refine_diff_density_rms         0.286
_refine_ls_extinction_coef       0.0045(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.074
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     128
_refine_ls_number_reflns         1455
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0591
_refine_ls_R_factor_gt           0.0504
_refine_ls_restrained_S_all      1.074
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+14.7949P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0963
_refine_ls_wR_factor_ref         0.1011
_refine_special_details          ?
_olex2_refinement_description    
;
1. Others
 Fixed Sof: O7(0.5)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.24520(10) 0.88876(18) 0.33544(8) 0.0165(3) Uani 1 1 d . . . . .
Cd1 Cd 0.42422(7) 0.42415(13) 0.13337(6) 0.0117(2) Uani 1 1 d . . . . .
Cd2 Cd 0.09103(7) 0.40785(15) 0.13526(7) 0.0213(3) Uani 1 1 d . . . . .
B1 B 0.3989(10) 0.414(2) 0.4065(9) 0.012(2) Uani 1 1 d . . . . .
B2 B 0.2788(11) -0.069(2) 0.0878(10) 0.016(2) Uani 1 1 d . . . . .
B3 B -0.0520(11) 0.902(2) 0.0917(10) 0.019(2) Uani 1 1 d . . . . .
O1 O 0.3248(8) 0.5684(15) 0.4765(6) 0.0271(19) Uani 1 1 d . . . . .
O2 O 0.4501(7) 0.5477(14) 0.3199(6) 0.0173(15) Uani 1 1 d . . . . .
O3 O 0.5855(7) 0.6641(13) 0.0704(5) 0.0138(14) Uani 1 1 d . . . . .
O4 O 0.2644(7) 0.1460(13) 0.1523(6) 0.0151(15) Uani 1 1 d . . . . .
O5 O 0.2493(7) 0.6975(13) 0.1300(6) 0.0192(15) Uani 1 1 d . . . . .
O6 O -0.0831(10) 0.6587(19) 0.0842(12) 0.061(4) Uani 1 1 d . . . . .
O7 O 0.004(2) 1.069(3) 0.0173(15) 0.038(5) Uani 0.5 1 d . . P . .
O8 O 0.0684(11) 0.563(2) 0.3204(9) 0.061(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sr1 Cd1 3.5429(13) 2_655 ?
Sr1 B1 3.300(12) 1_565 ?
Sr1 B2 3.373(11) 4_566 ?
Sr1 B2 2.905(11) 1_565 ?
Sr1 B3 3.411(13) 2_545 ?
Sr1 O1 2.472(8) . ?
Sr1 O2 2.841(8) . ?
Sr1 O3 2.530(7) 2_655 ?
Sr1 O4 2.526(7) 1_565 ?
Sr1 O5 2.579(8) . ?
Sr1 O6 2.449(11) 2 ?
Sr1 O8 2.552(10) . ?
Cd1 Sr1 3.5428(13) 2_645 ?
Cd1 Sr1 3.9973(12) 4_575 ?
Cd1 O2 2.440(7) 2_645 ?
Cd1 O2 2.258(7) . ?
Cd1 O3 2.398(6) 3_665 ?
Cd1 O3 2.277(7) . ?
Cd1 O4 2.265(7) . ?
Cd1 O5 2.357(7) . ?
Cd2 Sr1 4.0354(13) 4_575 ?
Cd2 Sr1 3.6235(14) 2_545 ?
Cd2 Sr1 3.9010(13) 1_545 ?
Cd2 O4 2.310(7) . ?
Cd2 O5 2.278(8) . ?
Cd2 O6 2.338(10) . ?
Cd2 O6 2.558(14) 3_565 ?
Cd2 O7 2.405(15) 1_545 ?
Cd2 O8 2.310(12) . ?
Cd2 O8 2.553(14) 2_545 ?
B1 Sr1 3.300(11) 1_545 ?
B1 O1 1.410(13) . ?
B1 O2 1.355(12) . ?
B1 O3 1.349(13) 2_645 ?
B2 Sr1 3.373(11) 4_565 ?
B2 Sr1 2.905(11) 1_545 ?
B2 O1 1.393(13) 4_565 ?
B2 O4 1.365(13) . ?
B2 O5 1.362(13) 1_545 ?
B3 Sr1 3.411(13) 2 ?
B3 O6 1.325(16) . ?
B3 O7 1.38(2) 3_575 ?
B3 O7 1.38(2) . ?
B3 O8 1.336(15) 2 ?
O1 B2 1.393(13) 4_566 ?
O2 Cd1 2.440(7) 2_655 ?
O3 Sr1 2.530(7) 2_645 ?
O3 Cd1 2.398(6) 3_665 ?
O3 B1 1.349(13) 2_655 ?
O4 Sr1 2.526(7) 1_545 ?
O5 B2 1.362(13) 1_565 ?
O6 Sr1 2.449(11) 2_545 ?
O6 Cd2 2.558(14) 3_565 ?
O7 Cd2 2.405(15) 1_565 ?
O7 B3 1.38(2) 3_575 ?
O7 O7 0.83(3) 3_575 ?
O8 Cd2 2.553(14) 2 ?
O8 B3 1.336(15) 2_545 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
B1 Sr1 Cd1 56.32(19) 1_565 2_655 ?
B1 Sr1 B2 99.5(3) 1_565 4_566 ?
B1 Sr1 B3 149.9(3) 1_565 2_545 ?
B2 Sr1 Cd1 82.2(2) 4_566 2_655 ?
B2 Sr1 Cd1 86.4(2) 1_565 2_655 ?
B2 Sr1 B1 95.9(3) 1_565 1_565 ?
B2 Sr1 B2 151.2(2) 1_565 4_566 ?
B2 Sr1 B3 57.3(3) 4_566 2_545 ?
B2 Sr1 B3 113.5(3) 1_565 2_545 ?
B3 Sr1 Cd1 128.7(2) 2_545 2_655 ?
O1 Sr1 Cd1 69.6(2) . 2_655 ?
O1 Sr1 B1 104.5(3) . 1_565 ?
O1 Sr1 B2 130.5(3) . 1_565 ?
O1 Sr1 B2 21.2(3) . 4_566 ?
O1 Sr1 B3 61.5(3) . 2_545 ?
O1 Sr1 O2 50.6(2) . . ?
O1 Sr1 O3 83.3(3) . 2_655 ?
O1 Sr1 O4 151.7(2) . 1_565 ?
O1 Sr1 O5 108.9(2) . . ?
O1 Sr1 O8 79.8(3) . . ?
O2 Sr1 Cd1 43.23(15) . 2_655 ?
O2 Sr1 B1 99.5(2) . 1_565 ?
O2 Sr1 B2 82.1(3) . 1_565 ?
O2 Sr1 B2 71.5(2) . 4_566 ?
O2 Sr1 B3 91.0(3) . 2_545 ?
O3 Sr1 Cd1 39.82(15) 2_655 2_655 ?
O3 Sr1 B1 22.1(2) 2_655 1_565 ?
O3 Sr1 B2 82.1(3) 2_655 4_566 ?
O3 Sr1 B2 105.5(3) 2_655 1_565 ?
O3 Sr1 B3 138.8(2) 2_655 2_545 ?
O3 Sr1 O2 81.2(2) 2_655 . ?
O3 Sr1 O5 125.6(2) 2_655 . ?
O3 Sr1 O8 158.3(3) 2_655 . ?
O4 Sr1 Cd1 86.86(17) 1_565 2_655 ?
O4 Sr1 B1 72.9(2) 1_565 1_565 ?
O4 Sr1 B2 169.0(3) 1_565 4_566 ?
O4 Sr1 B2 28.0(3) 1_565 1_565 ?
O4 Sr1 B3 132.6(3) 1_565 2_545 ?
O4 Sr1 O2 101.4(2) 1_565 . ?
O4 Sr1 O3 88.6(2) 1_565 2_655 ?
O4 Sr1 O5 55.5(2) 1_565 . ?
O4 Sr1 O8 112.7(3) 1_565 . ?
O5 Sr1 Cd1 93.59(18) . 2_655 ?
O5 Sr1 B1 122.0(2) . 1_565 ?
O5 Sr1 B2 126.6(2) . 4_566 ?
O5 Sr1 B2 28.0(3) . 1_565 ?
O5 Sr1 B3 88.1(3) . 2_545 ?
O5 Sr1 O2 69.9(2) . . ?
O6 Sr1 Cd1 130.4(2) 2 2_655 ?
O6 Sr1 B1 76.9(3) 2 1_565 ?
O6 Sr1 B2 90.9(4) 2 4_566 ?
O6 Sr1 B2 116.4(4) 2 1_565 ?
O6 Sr1 B3 84.1(3) 2 2_545 ?
O6 Sr1 O1 112.1(4) 2 . ?
O6 Sr1 O2 161.4(3) 2 . ?
O6 Sr1 O3 90.6(3) 2 2_655 ?
O6 Sr1 O4 95.1(3) 2 1_565 ?
O6 Sr1 O5 127.7(3) 2 . ?
O6 Sr1 O8 83.2(4) 2 . ?
O8 Sr1 Cd1 140.8(3) . 2_655 ?
O8 Sr1 B1 159.9(4) . 1_565 ?
O8 Sr1 B2 95.9(3) . 1_565 ?
O8 Sr1 B2 77.2(3) . 4_566 ?
O8 Sr1 B3 20.0(3) . 2_545 ?
O8 Sr1 O2 98.2(3) . . ?
O8 Sr1 O5 73.4(3) . . ?
Sr1 Cd1 Sr1 122.94(2) 2_645 4_575 ?
O2 Cd1 Sr1 142.1(2) . 4_575 ?
O2 Cd1 Sr1 129.17(16) 2_645 4_575 ?
O2 Cd1 Sr1 80.3(2) . 2_645 ?
O2 Cd1 Sr1 52.87(19) 2_645 2_645 ?
O2 Cd1 O2 88.58(18) . 2_645 ?
O2 Cd1 O3 94.5(2) . . ?
O2 Cd1 O3 172.7(2) . 3_665 ?
O2 Cd1 O4 99.2(2) . . ?
O2 Cd1 O5 84.8(3) . . ?
O3 Cd1 Sr1 86.12(17) . 4_575 ?
O3 Cd1 Sr1 45.38(18) . 2_645 ?
O3 Cd1 Sr1 95.50(17) 3_665 2_645 ?
O3 Cd1 Sr1 36.92(17) 3_665 4_575 ?
O3 Cd1 O2 93.6(2) 3_665 2_645 ?
O3 Cd1 O2 95.9(3) . 2_645 ?
O3 Cd1 O3 78.4(3) . 3_665 ?
O3 Cd1 O5 105.5(3) . . ?
O4 Cd1 Sr1 84.46(17) . 4_575 ?
O4 Cd1 Sr1 135.17(17) . 2_645 ?
O4 Cd1 O2 82.3(2) . 2_645 ?
O4 Cd1 O3 166.2(2) . . ?
O4 Cd1 O3 88.0(2) . 3_665 ?
O4 Cd1 O5 78.1(2) . . ?
O5 Cd1 Sr1 58.82(18) . 4_575 ?
O5 Cd1 Sr1 145.20(18) . 2_645 ?
O5 Cd1 O2 158.0(3) . 2_645 ?
O5 Cd1 O3 95.6(3) . 3_665 ?
Sr1 Cd2 Sr1 121.13(3) 1_545 4_575 ?
Sr1 Cd2 Sr1 121.73(3) 2_545 4_575 ?
Sr1 Cd2 Sr1 108.88(3) 2_545 1_545 ?
O4 Cd2 Sr1 140.40(18) . 2_545 ?
O4 Cd2 Sr1 38.14(16) . 1_545 ?
O4 Cd2 Sr1 83.04(16) . 4_575 ?
O4 Cd2 O6 90.0(3) . 3_565 ?
O4 Cd2 O6 170.2(4) . . ?
O4 Cd2 O7 84.1(6) . 1_545 ?
O4 Cd2 O8 95.7(3) . 2_545 ?
O4 Cd2 O8 104.1(3) . . ?
O5 Cd2 Sr1 100.68(19) . 1_545 ?
O5 Cd2 Sr1 58.17(19) . 4_575 ?
O5 Cd2 Sr1 139.56(19) . 2_545 ?
O5 Cd2 O4 78.8(3) . . ?
O5 Cd2 O6 93.6(3) . 3_565 ?
O5 Cd2 O6 101.6(3) . . ?
O5 Cd2 O7 138.5(4) . 1_545 ?
O5 Cd2 O8 83.8(3) . . ?
O5 Cd2 O8 169.0(3) . 2_545 ?
O6 Cd2 Sr1 42.0(3) . 2_545 ?
O6 Cd2 Sr1 88.9(3) . 4_575 ?
O6 Cd2 Sr1 119.3(2) 3_565 1_545 ?
O6 Cd2 Sr1 35.4(2) 3_565 4_575 ?
O6 Cd2 Sr1 149.1(3) . 1_545 ?
O6 Cd2 Sr1 95.3(2) 3_565 2_545 ?
O6 Cd2 O6 80.3(5) . 3_565 ?
O6 Cd2 O7 89.4(6) . 1_545 ?
O6 Cd2 O8 85.4(3) . 2_545 ?
O7 Cd2 Sr1 70.8(5) 1_545 2_545 ?
O7 Cd2 Sr1 82.6(4) 1_545 4_575 ?
O7 Cd2 Sr1 87.9(5) 1_545 1_545 ?
O7 Cd2 O6 48.7(5) 1_545 3_565 ?
O7 Cd2 O8 48.9(4) 1_545 2_545 ?
O8 Cd2 Sr1 77.5(3) . 2_545 ?
O8 Cd2 Sr1 44.8(2) 2_545 2_545 ?
O8 Cd2 Sr1 139.6(2) . 4_575 ?
O8 Cd2 Sr1 75.8(3) . 1_545 ?
O8 Cd2 Sr1 69.8(2) 2_545 1_545 ?
O8 Cd2 Sr1 131.1(2) 2_545 4_575 ?
O8 Cd2 O6 96.0(3) 2_545 3_565 ?
O8 Cd2 O6 85.7(5) . . ?
O8 Cd2 O6 164.9(4) . 3_565 ?
O8 Cd2 O7 137.2(5) . 1_545 ?
O8 Cd2 O8 88.3(3) . 2_545 ?
O1 B1 Sr1 109.8(7) . 1_545 ?
O2 B1 Sr1 117.5(6) . 1_545 ?
O2 B1 O1 112.1(9) . . ?
O3 B1 Sr1 44.9(5) 2_645 1_545 ?
O3 B1 O1 121.0(9) 2_645 . ?
O3 B1 O2 126.9(9) 2_645 . ?
Sr1 B2 Sr1 143.1(4) 1_545 4_565 ?
O1 B2 Sr1 39.9(5) 4_565 4_565 ?
O1 B2 Sr1 165.8(8) 4_565 1_545 ?
O4 B2 Sr1 150.9(7) . 4_565 ?
O4 B2 Sr1 60.3(5) . 1_545 ?
O4 B2 O1 123.6(9) . 4_565 ?
O5 B2 Sr1 80.9(6) 1_545 4_565 ?
O5 B2 Sr1 62.6(5) 1_545 1_545 ?
O5 B2 O1 115.2(9) 1_545 4_565 ?
O5 B2 O4 121.2(9) 1_545 . ?
O6 B3 Sr1 126.0(8) . 2 ?
O6 B3 O7 133.4(13) . . ?
O6 B3 O7 98.3(12) . 3_575 ?
O6 B3 O8 128.3(13) . 2 ?
O7 B3 Sr1 87.7(9) . 2 ?
O7 B3 Sr1 113.0(11) 3_575 2 ?
O7 B3 O7 35.1(12) . 3_575 ?
O8 B3 Sr1 40.7(6) 2 2 ?
O8 B3 O7 98.3(11) 2 . ?
O8 B3 O7 133.4(13) 2 3_575 ?
B1 O1 Sr1 101.6(6) . . ?
B2 O1 Sr1 118.9(7) 4_566 . ?
B2 O1 B1 139.0(9) 4_566 . ?
Cd1 O2 Sr1 83.9(2) 2_655 . ?
Cd1 O2 Sr1 100.1(3) . . ?
Cd1 O2 Cd1 119.4(3) . 2_655 ?
B1 O2 Sr1 87.0(6) . . ?
B1 O2 Cd1 121.2(6) . . ?
B1 O2 Cd1 119.4(6) . 2_655 ?
Cd1 O3 Sr1 108.4(3) 3_665 2_645 ?
Cd1 O3 Sr1 94.8(2) . 2_645 ?
Cd1 O3 Cd1 101.6(3) . 3_665 ?
B1 O3 Sr1 113.0(6) 2_655 2_645 ?
B1 O3 Cd1 124.4(6) 2_655 . ?
B1 O3 Cd1 112.5(6) 2_655 3_665 ?
Cd1 O4 Sr1 120.8(3) . 1_545 ?
Cd1 O4 Cd2 102.3(3) . . ?
Cd2 O4 Sr1 107.5(3) . 1_545 ?
B2 O4 Sr1 91.6(6) . 1_545 ?
B2 O4 Cd1 112.3(6) . . ?
B2 O4 Cd2 123.6(7) . . ?
Cd1 O5 Sr1 105.3(3) . . ?
Cd2 O5 Sr1 101.4(3) . . ?
Cd2 O5 Cd1 100.5(3) . . ?
B2 O5 Sr1 89.4(6) 1_565 . ?
B2 O5 Cd1 111.2(7) 1_565 . ?
B2 O5 Cd2 142.5(7) 1_565 . ?
Sr1 O6 Cd2 107.4(4) 2_545 3_565 ?
Cd2 O6 Sr1 98.4(4) . 2_545 ?
Cd2 O6 Cd2 99.7(5) . 3_565 ?
B3 O6 Sr1 135.6(10) . 2_545 ?
B3 O6 Cd2 109.4(8) . . ?
B3 O6 Cd2 101.3(9) . 3_565 ?
B3 O7 Cd2 106.6(10) . 1_565 ?
B3 O7 Cd2 106.8(10) 3_575 1_565 ?
B3 O7 B3 144.9(12) . 3_575 ?
O7 O7 Cd2 162(4) 3_575 1_565 ?
O7 O7 B3 73(2) 3_575 . ?
O7 O7 B3 72(2) 3_575 3_575 ?
Sr1 O8 Cd2 90.5(4) . 2 ?
Cd2 O8 Sr1 101.3(4) . . ?
Cd2 O8 Cd2 122.0(4) . 2 ?
B3 O8 Sr1 119.3(8) 2_545 . ?
B3 O8 Cd2 100.9(9) 2_545 2 ?
B3 O8 Cd2 120.1(9) 2_545 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Sr1 B1 O1 Sr1 -101.4(4) 1_545 . . . ?
Sr1 B1 O1 B2 69.7(15) 1_545 . . 4_566 ?
Sr1 B1 O2 Sr1 102.4(5) 1_545 . . . ?
Sr1 B1 O2 Cd1 2.5(9) 1_545 . . . ?
Sr1 B1 O2 Cd1 -176.4(3) 1_545 . . 2_655 ?
Sr1 B2 O4 Sr1 150.4(14) 4_565 . . 1_545 ?
Sr1 B2 O4 Cd1 -85.2(15) 4_565 . . . ?
Sr1 B2 O4 Cd1 124.4(5) 1_545 . . . ?
Sr1 B2 O4 Cd2 38.1(18) 4_565 . . . ?
Sr1 B2 O4 Cd2 -112.3(6) 1_545 . . . ?
Sr1 B3 O6 Sr1 -22.6(17) 2 . . 2_545 ?
Sr1 B3 O6 Cd2 107.2(8) 2 . . 3_565 ?
Sr1 B3 O6 Cd2 -148.1(5) 2 . . . ?
Sr1 B3 O7 Cd2 61.3(9) 2 . . 1_565 ?
Sr1 B3 O7 B3 -137(3) 2 . . 3_575 ?
Sr1 B3 O7 O7 -137(3) 2 . . 3_575 ?
O1 B1 O2 Sr1 -26.1(8) . . . . ?
O1 B1 O2 Cd1 55.1(10) . . . 2_655 ?
O1 B1 O2 Cd1 -126.1(8) . . . . ?
O1 B2 O4 Sr1 -164.0(11) 4_565 . . 1_545 ?
O1 B2 O4 Cd1 -39.6(13) 4_565 . . . ?
O1 B2 O4 Cd2 83.7(12) 4_565 . . . ?
O2 B1 O1 Sr1 31.1(9) . . . . ?
O2 B1 O1 B2 -157.9(12) . . . 4_566 ?
O3 B1 O1 Sr1 -149.9(8) 2_645 . . . ?
O3 B1 O1 B2 21(2) 2_645 . . 4_566 ?
O3 B1 O2 Sr1 154.9(10) 2_645 . . . ?
O3 B1 O2 Cd1 55.0(13) 2_645 . . . ?
O3 B1 O2 Cd1 -123.8(10) 2_645 . . 2_655 ?
O5 B2 O4 Sr1 15.4(11) 1_545 . . 1_545 ?
O5 B2 O4 Cd1 139.8(9) 1_545 . . . ?
O5 B2 O4 Cd2 -96.9(11) 1_545 . . . ?
O6 B3 O7 Cd2 -158.2(12) . . . 1_565 ?
O6 B3 O7 B3 3(4) . . . 3_575 ?
O6 B3 O7 O7 3(4) . . . 3_575 ?
O7 B3 O6 Sr1 -149.0(14) 3_575 . . 2_545 ?
O7 B3 O6 Sr1 -150.8(17) . . . 2_545 ?
O7 B3 O6 Cd2 -21(2) . . . 3_565 ?
O7 B3 O6 Cd2 85.4(13) 3_575 . . . ?
O7 B3 O6 Cd2 84(2) . . . . ?
O7 B3 O6 Cd2 -19.2(13) 3_575 . . 3_565 ?
O7 B3 O7 Cd2 -161(4) 3_575 . . 1_565 ?
O7 B3 O7 B3 0.001(2) 3_575 . . 3_575 ?
O8 B3 O6 Sr1 29(2) 2 . . 2_545 ?
O8 B3 O6 Cd2 -96.5(14) 2 . . . ?
O8 B3 O6 Cd2 158.8(12) 2 . . 3_565 ?
O8 B3 O7 Cd2 21.9(13) 2 . . 1_565 ?
O8 B3 O7 B3 -177(3) 2 . . 3_575 ?
O8 B3 O7 O7 -177(3) 2 . . 3_575 ?

_olex2_submission_special_instructions 'No special instructions were received'
